 Nano Express
 Open Access
 Published:
Nanoindentation experiments for singlelayer rectangular graphene films: a molecular dynamics study
Nanoscale Research Letters volume 9, Article number: 41 (2014)
 The Erratum to this article has been published in Nanoscale Research Letters 2014 9:228
Abstract
A molecular dynamics study on nanoindentation experiments is carried out for some singlelayer rectangular graphene films with four edges clamped. Typical load–displacement curves are obtained, and the effects of various factors including indenter radii, loading speeds, and aspect ratios of the graphene film on the simulation results are discussed. A formula describing the relationship between the load and indentation depth is obtained according to the molecular dynamics simulation results. Young’s modulus and the strength of the singlelayer graphene film are measured as about 1.0 TPa and 200 GPa, respectively. It is found that the graphene film ruptured in the central point at a critical indentation depth. The deformation mechanisms and dislocation activities are discussed in detail during the loadingunloadingreloading process. It is observed from the simulation results that once the loading speed is larger than the critical loading speed, the maximum force exerted on the graphene film increases and the critical indentation depth decreases with the increase of the loading speed.
Background
The perfect graphene is a kind of carbonaceous material which consists of twodimensional honeycomb lattice structures of single layer of carbon atoms. It is the basic unit to build other dimensional carbonaceous materials, such as zerodimensional fullerenes, onedimensional carbon nanotubes, and threedimensional graphite[1, 2]. Graphene sheets/ribbons/films have attracted the interest of the scientific community because of recent exciting experimental results[3–6]. Their growth, atomic makeup, electronics, doping, and intercalation have attracted many investigations[7–10]. A suspended graphene sheet[1, 11] can be used in a variety of ways, such as for pressure sensors or gas detectors[12] or mechanical resonators[13].
It is still debatable whether a graphene sheet is truly a twodimensional structure or if it should be regarded as a threedimensional structure since it exhibits a natural tendency to ripple, as observed in recent experiments[2, 14–16]. Carlsson addressed that an understanding of the coupling behaviors between bending and stretching of graphene sheets is necessary to fully explain the intrinsic ripples in a graphene sheet[15]. In addition to theoretical investigations, recent research has been carried out to measure the mechanical properties of suspended graphene sheets by utilizing an atomic force microscope (AFM)[17]. Through weak van der Waals forces, graphene sheets were suspended over silicon dioxide cavities where an AFM tip was probed to test its mechanical properties. Their Young’s modulus differs from that of bulk graphite. Poot and van der Zan[18] measured the nanomechanical properties of graphene sheets suspended over circular holes by using an AFM and suggested that graphene sheets can sustain very large bending and stretching prior to the occurrence of fracture, which indicates that the classical Kirchhoff plate theory used in the bending and vibration analysis of graphene sheets may not be suitable since deflection and stretching are considerable[19]. Some researchers thought that the large deflection plate theory of von Kármán may be a better candidate to model the graphene sheet, and they have characterized its bending and stretching through that theory[20, 21]. Lee et al. measured Young’s modulus and the maximum stress of graphene by using an AFM in the nanoindentation experiment[22] and reported the effect of grain boundaries on the measurement of chemical vapordeposited graphene[23]. Fang et al.[24] has studied the mechanical behavior of a rectangular graphene film under various indentation depths, velocities, and temperatures using molecular dynamics (MD) simulations. The physical models of the rectangular graphene film established by Fang et al. are doubly clamped using a bridgetype support and are loaded by a flatbottomed diamond tip.
Although the above research has been carried out for mechanical properties of graphene, the variation of the values of elastic modulus has not yet reached a consensus. Especially for rectangular graphene films, the relationship between the load and the indentation depth is not clear. Furthermore, there are few papers available which describe the deformation mechanisms and dislocation activities of graphene film during the nanoindentation processes in detail. These investigations are concentrated on tension deformation[25–28] and shear deformation[29]. Almost all of the available literatures on dislocation activities in graphene focus on theoretical studies and numerical simulations, including density functional theory (DFT)[26], tightbinding molecular dynamics (TBMD)[30], ab initio total energy calculation[30], and quantum mechanical computations[31]. Researchers always artificially applied defects or dislocations and then studied their effects on the properties and activities in graphene. However, due to the bottleneck of experimental study at nanoscale, a very few experimental observations of dislocation activities are available at present. Warner et al.[32] also reported the observation of dislocation pairs through HRTEM experiments and gave five possible mechanisms that describe how these dislocation pairs could have formed, namely, during the CVD growth, electron beam sputtering of carbon dimers along a zigzag lattice direction, from surface adatom incorporation, from a monovacancy, and from a StoneWales defect. They then concluded that edge dislocations result in substantial deformation of the atomic structure of graphene, with bond compression or elongation of ±27%, plus shear strain and lattice rotations.
In this article, some MD simulations of nanoindentation experiments are performed on a set of singlelayer rectangular graphene films with four clamped edges. The dislocation activities and the deformation mechanism are discussed, and a formula is introduced in order to describe the relationship of load and indentation depth and to measure the mechanical properties of graphene.
Methods
In order to carry out the nanoindentation experiments, one diamond sphere was introduced to simulate the indenter. Figure 1a shows the origin model for the nanoindentation experiment. Here, the upper ball is the indenter and constructed by diamond, which is considered as a rigid object so that the atomic configuration of the diamond indenter had no changes during MD simulations. The lower plane is a singlelayer rectangular graphene film with different aspect ratios. For the inner atoms of the indenter and the graphene film, the energy function was described by adaptive intermolecular reactive empirical bond order (AIREBO) potential. Compared with the TersoffBrenner potential, the AIREBO potential not only introduces multibody potential effects and the local atomic circumstance effect but also adds longrange interactions and a torsion term[33], and it has been found be more suitable than the Tersofftype potential for accurately capturing Young’s modulus of graphene as well as bond breaking and reforming between carbon atoms[28]. In order to avoid the influence of nonphysical explanations with improper cutoff functions on the fracture process, the cutoff parameter of the AIREBO potential is set to be 2.0 Å. As for the interaction between the indenter and the graphene film, van der Waals forces were simulated based on the LennardJones potential.
When performing MD simulations, we use the canonical (i.e., NVT) ensemble and control the temperatures at an ideal temperature of 0.01 K. In order to avoid the complex effects of the atomic thermal fluctuations, the temperature is regulated with the NoséHoover method and the time step was set to 1 fs. During the simulation, one key step, named energy minimization and relaxation, should be carried out to make the system remain in the equilibrium state with lowest energy. Then, the indentation experiment was executed and the simulation results were output for further research.
Results and discussion
Loading and unloading properties
We take the case of the graphene film with an aspect ratio of 1.2 and the diamond indenter with a radius of 2 nm as an example to describe the indentation experiment in the following. The indenter was placed over the geometric center of the graphene film and forced to move in the direction perpendicular to the original graphene surface. Figure 1 gives the atomic configurations of the system model during the indentation experiment at a speed of 0.20 Å/ps. The atoms on the edge of the graphene film remained in a static state due to fixed boundary conditions. After enough loading time, the graphene film is eventually pierced through by the indenter, appearing some fractured graphene lattices. The load–displacement curves can be attained from the data of intender load (F) and indentation depth (d) calculated in MD simulations. The moment the load–displacement curve drops suddenly is considered to be a critical moment. In our simulations, the load suddenly decreased once the indentation depth exceeded 5.595 nm, defined as the critical indentation depth (d_{c}), and the corresponding maximum load (F_{max}) is 655.08 nN.
Figure 2 gives some detailed views on the graphene lattice fracture process starting from the critical moment. It is shown in Figure 2a that the carbon network was expanded largely, but there is no broken carboncarbon (CC) bond at the critical moment. Figure 2b represents the moment the bondbroken phenomenon emerged for the first time, with a pore appearing. The bondbroken process is irreversible and the load exerted on the graphene firstly declines. The first appearance of the pentagonalheptagonal (5–7) and trilateral structures is shown in Figure 2c. Unlike with other StoneWales 5775 (SW) defects mentioned in[34–36], in our indentation simulations, the loads are applied in the direction perpendicular to the surface of the graphene film and the 5–7 structure seems not conjugate but singular. In addition, it is found that the trilateral structure is an interim state in the evolution process from a pristine hexagonal structure to the 5–7 structure. A 536 structure including this trilateral structure and its adjacent structures would evolve into another 5–7 structure, the right one in Figure 2d, through bond breaking and bond reforming. Furthermore, a singlechain structure, shown in Figure 2e, can be observed during the fracture process, which can also be found in[26]. Afterwards, the single chain was broken and the indenter totally pierced through the graphene film.
Generally speaking, elastic deformation which is reversible and plastic deformation which is irreversible are two typical kinds of deformation of an object or material in the view of engineering. In order to determine whether the deformation of the graphene film is elastic or plastic, a set of experiments of loadingunloadingreloading processes are conducted. As shown in Figure 3, during the continuous loading process of the indenter on the graphene film, it can be found that the graphene film mainly takes on two stages in sequence:

Stage I. The unloading process is done before the indentation depth reaches the critical depth, d_{c}. The graphene sheet almost can make a complete recovery, i.e., restore its initial structures, and the curves of reloading processes almost perfectly match the initial loading curve while the unloading curve shows very small deviations from the initial one, as shown in the inset of Figure 3. In general, the almostperfect coincidence is due to the fact that the carbon covalent bonds and the graphene lattice structure are not destroyed. It can be concluded that there is no plastic deformation in this stage, i.e., the graphene undergoes elastic deformation.

Stage II, i.e., the yellow region in Figure 3. In Figure 4a,b,c, it is after the indentation depth exceeded d_{c} that the unloading process begins. The graphene sheet cannot make a complete recovery, and there exited broken covalent bonds after the unloading process. In the reloading process, the maximum force exerting on graphene is much smaller than that in Figure 3, which denotes the fracture of graphene lattices. Figure 4b describes the state where the unloading process begins, and Figure 4c describes the state where the unloading process ends. After the loading process, there exited broken bonds and fractured lattices in the middle of the graphene film and these defective structures did not recover during the unloading process. Therefore, the deformation of the graphene described in this figure can be considered as a plastic type.
Young’s modulus and strength of the graphene film
According to the available correlation for the indentation experiments of a circular singlelayer graphene film in[18, 22, 37], one new formula is constructed to describe the relationship between indention depth and load,
where d is the indentation depth and F denotes the concentrated force gotten by the graphene film. In Equation 1, the load F consists of two parts: the first part, F_{ σ }(d), represents the term due to the axial tension of the twodimensional (2D) film,
where σ_{0}^{2D} is the pretension of the singlelayer graphene film, r is the indenter radius, β denotes the aspect ratio and is equal to L/b, and R_{equ} represents the equivalent radius of the rectangular graphene sheet, (Lb/π)^{1/2}. The second one, F_{E}(d), represents the large deformation term,
where E^{2D} is the 2D elastic modulus, i.e., Young’s modulus, of the single layer graphene film. The strain energy density of graphene, as a standard 2D material, can be represented by the energy of per unit area. Then, the corresponding pretension and elastic modulus can be expressed as σ_{0}^{2D} and E^{2D}, respectively, with the unit N/m. The common pretension and elastic modulus of a 3D bulk material can be obtained through these 2D values divided respectively by the effective thickness which is always treated as the layer spacing of the graphite crystal, i.e., 3.35 Å. q is an nondimensional value, q = 1/(1.05  0.15ν  0.16ν^{2}) = 0.9795, where ν denotes Poisson’s ratio, ν = 0.165[3, 18, 21]. It is reported that when r/R > 0.1, the indenter radius has a significant influence on the load–displacement properties[38, 39]. In our simulations, r/R > 0.1; thus, Equations 2 and 3 are corrected by a factor of (r/R)^{3/4} and (r/R)^{1/4}, respectively.
According to the expression of maximum stress in the plane of a circular elastic film in[40], the maximum stress for a rectangular elastic film can be expressed by the following formula:
Figure 5 presents the curves of indentation depth versus load for the nanoindentation experiment. The red solid curve is from the MD simulation results. According to Equation 1, nonlinear least squares method was used to fit the simulation results, and then the black curve in Figure 5 can be obtained. It is noted that when the indentation depth is about 5.597 nm, the load received by the graphene film suddenly drops from approximately 655.08 to approximately 522.172 nN. Corresponding to Figure 2b,c, the lengths of CC bonds under the indenter quickly become larger than before, which indicates that the bonds were broken.
Table 1 gives the mechanical properties calculated from the MD simulation results. Young’s modulus and the maximum stress of the graphene are obtained as 1.0539 TPa and 205.1328 GPa, respectively. Young’s modulus obtained in this paper is in good agreement with those obtained by both experimental and numerical methods. Kudin et al. has predicted a Young’s modulus of 1.02 TPa using ab initio methods[41]. Lee et al. obtained a Young’s modulus of 1 ± 0.1 TPa by nanoindentation in an AFM of freestanding monolayer circular graphene membranes[22]. NeekAmal and Peeters studied the nanoindentation of a bilayer graphene using molecular dynamics simulations and estimated a Young’s modulus of 0.8 TPa[42]. In addition, the maximum stress ranges from 130 to 240 GPa by means of both experiments and numerical simulations reported in other literatures[21, 22, 43, 44]. The maximum stress obtained in this paper can also be included in the above range, which verified our simulation results. The changing trend of 2D pretension demonstrates that the pretension of the rectangular graphene film is positively correlated with the loading speed of the indenter. The indenter size also affects the pretension, which, to some extent, explains why the correction factors were introduced in Equations 2 and 3.
Other parameters’ influences on nanoindentation experiments
For further study of nanoindentation properties, a series of simulations have been carried out with different loading speeds, indenter radii, and aspect ratios of graphene film. It is indicated that the speed of 0.20 Å/ps can be regarded as the critical loading speed, as shown in Figure 6a. When the loading speed is higher than the critical value, with the increase of speed, the maximum load increases rapidly; simultaneously, the critical indentation depth decreases rapidly. However, when the loading speed is lower than the critical value, the changes of F_{max} and d_{ c } are not that obvious. When the loading speed decreases from 1.00 to 0.50 Å/ps, dropping by 50%, the value of d_{c} increases by 33.35%, and the value of F_{max} decreases by 8.43% correspondingly. Nevertheless, when the loading speed decreases from 0.20 to 0.10 Å/ps, dropping by 50%, the changes of F_{max} and d_{c} are only 1.68% and 0.21%, respectively. The results may be attributed to the fact that the higher the loading speed of the indenter, the less time it takes to go through the graphene sheet, resulting in a higher load and lower indentation depth than those at a lower loading speed, in which situation the load process is much slower. Secondarily, the spherical indenter’s influences on results are observed by changing the indenter radius. The simulations of various indenter radii (1, 2, and 3 nm) are carried out at the speed of 0.20 Å/ps. The results of the load–displacement curve are shown in Figure 6b. The stress is more uniform in the middle of the graphene, so the F_{max} increases obviously and the critical indentation depth also becomes greater with the increase of the indenter radius. Finally, after changing the aspect ratio of the graphene film to 1.1 and 1.5, Young’s modulus and the maximum stress of the graphene are obtained using the methods mentioned above. It can be deduced from Figure 7 that Young’s modulus and the maximum stress are the inherent properties of graphene and irrelevant to its size, which also verifies the formula obtained above.
Conclusions
Some MD simulations of nanoindentation experiments on singlelayer rectangular graphene sheets have been carried out in order to obtain the mechanical properties of graphene. A correlation between the load and the indentation depth is constructed, and Young’s modulus and the strength of graphene are obtained in the end. The simulation results show that the unloaded graphene film could make a complete recovery if the maximum indentation depth is less than the critical indentation depth, and the graphene film undergoes elastic deformation during the whole loadingunloadingreloading process. However, if the maximum indentation depth is larger than the critical indentation depth, the graphene sheet could not restore its original structures after unloading and the graphene deforms plastically. Based on the simulations of nanoindentation at different loading speeds and indenter radii, it can be observed that the maximum load increased and the critical indentation depth decreased with the increase of loading speed. In addition, the indenter radius has a remarkable influence on the forcedisplacement curve. As the indenter radius increases, the critical load and the critical indentation depth also increase.
Abbreviations
 2D:

twodimensional
 AFM:

atomic force microscope
 AIREBO:

adaptive intermolecular reactive empirical bond order
 GPa:

gigapascals
 MD:

molecular dynamics
 NVT:

constant number of particles, volume, and temperature
 SW:

StoneWales 5775
 TPa:

terapascals.
References
 1.
Geim A, Novoselov K: The rise of graphene. Nat Mater 2007, 6: 183–191. 10.1038/nmat1849
 2.
Wang W, Hao Y, Yi C, Ji X, Niu X: Relaxation properties of graphene nanoribbons at different ambient temperatures: a molecular dynamics. Acta Phys Sin 2012, 61: 200207.
 3.
Novoselov K, Geim A, Morozov S, Jiang D, Zhang Y, Dubonos S, Grigorieva I, Firsov A: Electric field effect in atomically thin carbon films. Science 2004, 306: 666–669. 10.1126/science.1102896
 4.
Novoselov K, Jiang Z, Zhang Y, Morozov S, Stormer H, Zeitler U, Maan J, Boebinger G, Kim P, Geim A: Roomtemperature quantum hall effect in graphene. Science 2007, 315: 1397.
 5.
BarzolaQuiquia J, Esquinazi P, Rothermel M, Spemann D, Butz T, Garcia N: Experimental evidence for twodimensional magnetic order in proton bombarded graphite. Phys Rev B 2007, 76: 1403.
 6.
Peter W, JanIngo F, Eli A: Epitaxial graphene on ruthenium. Nat Mater 2008, 7: 406–411. 10.1038/nmat2166
 7.
Chiu Y, Lai Y, Ho J, Chuu D, Lin M: Electronic structure of a twodimensional graphene monolayer in a spatially modulated magnetic field: peierls tightbinding model. Phys Rev B 2008, 77: 045407.
 8.
Dutta S, Lakshmi S, Pati S: Electron–electron interactions on the edge states of graphene: a manybody configuration interaction study. Phys Rev B 2008, 77: 073412.
 9.
Lai Y, Ho J, Chang C, Lin M: Magnetoelectronic properties of bilayer Bernal graphene. Phys Rev B 2008, 77: 085426.
 10.
Lherbier A, Biel B, Niquet Y, Roche S: Transport length scales in disordered graphenebased materials: strong localization regimes and dimensionality effects. Phys Rev Lett 2008, 100: 036803.
 11.
Meyer J, Geim A, Katsnelson M, Novoselov K, Booth T, Roth S: The structure of suspended graphene sheets. Nature 2007, 446: 60–63. 10.1038/nature05545
 12.
Schedin F, Geim A, Morozov S, Hill E, Blake P, Katsnelson M, Novoselov K: Detection of individual gas molecules adsorbed on graphene. Nat Mater 2007, 6: 652–655. 10.1038/nmat1967
 13.
Bunch J, van der Zande A, Verbridge S, Frank I, Tanenbaum D, Parpia J, Craighead H, McEuen P: Electromechanical resonators from graphene sheets. Science 2007, 315: 490–493. 10.1126/science.1136836
 14.
Fasolino A, Los J, Katsnelson M: Intrinsic ripples in graphene. Nat Mater 2007, 6: 858–861. 10.1038/nmat2011
 15.
Carlsson J: Graphene: buckle or break. Nat Mater 2007, 6: 801–802.
 16.
Zhou J, Huang R: Internal lattice relaxation of singlelayer graphene under inplane deformation. J Mech Phys Solids 2008, 56: 1609–1623. 10.1016/j.jmps.2007.07.013
 17.
Frank I, Tanenbaum D, van der Zande A, McEuen P: Mechanical properties of suspended graphene sheets. J Vac Sci Technol B 2007, 25: 2558–2561. 10.1116/1.2789446
 18.
Poot M, van der Zan H: Nanomechanical properties of fewlayer graphene membranes. Appl Phys Lett 2008, 92: 063111. 10.1063/1.2857472
 19.
Duan W, Wang C: Nonlinear bending and stretching of a circular graphene sheet under a central point load. Nanotechnology 2009, 20: 077702.
 20.
Landau L, Lifshits E: Theory of Elasticity. New York: Pergamon; 1970.
 21.
Yang X, He P, Wu A, Zheng B: Molecular dynamics simulation of nanoindentation for graphene. Scientia Sinica: Phys, Mech, Astron 2010, 40: 353–360.
 22.
Lee C, Wei X, Kysar J, Hone J: Measurement of the elastic properties and intrinsic strength of monolayer graphene. Science 2008, 321: 385–388. 10.1126/science.1157996
 23.
Lee G, Cooper R, An S, Lee S, Zande A, Petrone N, Hammerberg A, Lee C, Crawford B, Oliver W, Kysar J, Hone J: Highstrength chemicalvapor–deposited graphene and grain boundaries. Science 2013, 340: 1073–1076. 10.1126/science.1235126
 24.
Fang T, Wang T, Yang J, Hsiao Y: Mechanical characterization of nanoindented graphene via molecular dynamics simulations. Nanoscale Res Lett 2011, 6: 481. 10.1186/1556276X6481
 25.
Kiselev S, Zhirov E: Molecular dynamic simulation of deformation and fracture of graphene under uniaxial tension. Phys Mesomech 2013, 16: 125–132. 10.1134/S1029959913020033
 26.
Topsakal M, Ciraci S: Elastic and plastic deformation of graphene, silicene, and boron nitride honeycomb nanoribbons under uniaxial tension: a firstprinciples densityfunctional theory study. Phys Rev B 2010, 81: 024107.
 27.
Xu Z: Graphene nanoribbons under tension. J Comput Theor Nanos 2009, 6: 1–3. 10.1166/jctn.2009.1001
 28.
Zhao H, Min K, Aluru N: Size and chirality dependent elastic properties of graphene nanoribbons under uniaxial tension. Nano Lett 2009, 9: 3012. 10.1021/nl901448z
 29.
Carpio A, Bonilla L: Periodized discrete elasticity models for defects in graphene. Phys Rev B 2008, 78: 085406.
 30.
Lee G, Yoon E, Hwang N, Wang C, Ho K: Formation and development of dislocation in graphene. Appl Phys Lett 2013, 102: 021603. 10.1063/1.4775671
 31.
Dumitrica T, Hua M, Yakobson B: Symmetry, time, and temperaturedependent strength of carbon nanotubes. Proc Natl Acad Sci U S A 2006, 103: 6105–6109. 10.1073/pnas.0600945103
 32.
Warner J, Margine E, Mukai M, Robertson A, Giustino F, Kirkland A: Dislocationdriven deformations in graphene. Science 2012, 337: 209. 10.1126/science.1217529
 33.
Wang W, Yi C, Ji X, Niu X: Molecular dynamics study on relaxation characteristics of graphene nanoribbons at room temperature. Nanosci Nanotechnol Lett 2012, 4: 1188–1193. 10.1166/nnl.2012.1457
 34.
Zhao H, Aluru N: Temperature and strainrate dependent fracture strength of graphene. J Appl Phys 2010, 108: 064321. 10.1063/1.3488620
 35.
Xu L, Wei N, Zheng Y: Mechanical properties of highly defective graphene: from brittle rupture to ductile fracture. Nanotechnology 2013, 24: 505703. 10.1088/09574484/24/50/505703
 36.
Xiao J, Staniszewski J, Gillespie J Jr: Fracture and progressive failure of defective graphene sheets and carbon nanotubes. Compos Struct 2009, 88: 602–609. 10.1016/j.compstruct.2008.06.008
 37.
Komaragiri U, Begley M, Simmonds J: The mechanical response of freestanding circular elastic films on the point and pressure loads. J Apple Mech 2005, 72: 203–212. 10.1115/1.1827246
 38.
Begley M, Mackin T: Spherical indentation of freestanding circular thin films in the membrane regime. J Mech Phys Solid 2004, 52: 2005–2032. 10.1016/j.jmps.2004.03.002
 39.
Scott O, Begley M, Komaragiri U, Mackin T: Indentation of freestanding circular elastomer films using spherical indenters. Acta Mater 2004, 52: 4877–4885. 10.1016/j.actamat.2004.06.043
 40.
Bhatia N, Nachbar W: Finite indentation of elasticperfectly plastic membranes by a spherical indenter. AIAA J 1968, 6: 1050–1057. 10.2514/3.4672
 41.
Kudin K, Scuseria G, Yakobson B: C2F, BN, and C nanoshell elasticity from ab initio computations. Phys Rev B 2001, 64: 235406.
 42.
NeekAmal M, Peeters FM: Nanoindentation of a circular sheet of bilayer graphene. Phys Rev B 2010, 81: 235421.
 43.
Wu J, Hwang C, Huang Y: An atomistic based finite deformation shell theory for singlewall carbon nanotubes. J Mech Phys Solid 2008, 56: 279–292. 10.1016/j.jmps.2007.05.008
 44.
Lu Q, Arroyo M, Huang R: Elastic bending modulus of monolayer graphene. J Phys D Appl Phys 2009, 42: 245413.
Acknowledgements
We acknowledge the financial support provided by the Fundamental Research Funds for the Natural Science Basic Research Plan in Shaanxi Province of China (grant no. 2013JM7017), subsequently by the National Natural Science Foundations of China (grant no. 51205302 and no. 50903017) and the Central Universities in Xidian University (grant no. K5051304006). We also would like to thank all the reviewers for their comments and kind suggestions to our manuscript and all the editors for their careful corrections on the final version of the article.
Author information
Additional information
Competing interests
The authors declare that they have no competing interests.
Authors’ contributions
The analysis of the simulation results was mainly carried out by WDW. The simulation processes were mainly conducted by SL, JJM, and CLY. Some fairly helpful proposals about the construction of models were made by YJZ and MLL. All authors read and approved the final manuscript.
An erratum to this article can be found online at 10.1186/1556276X9228.
An erratum to this article is available at http://dx.doi.org/10.1186/1556276X9228.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 2.0 International License (https://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
About this article
Cite this article
Wang, W., Li, S., Min, J. et al. Nanoindentation experiments for singlelayer rectangular graphene films: a molecular dynamics study. Nanoscale Res Lett 9, 41 (2014). https://doi.org/10.1186/1556276X941
Received:
Accepted:
Published:
Keywords
 Molecular dynamics simulation
 Nanoindentation
 Rectangular graphene film
 Young’s modulus
 Strength